Upload
others
View
6
Download
0
Embed Size (px)
Citation preview
Cite this: RSC Advances, 2013, 3, 823
Chirality-dependent properties of carbon nanotubes:electronic structure, optical dispersion properties,Hamaker coefficients and van der Waals–Londondispersion interactions
Received 13th January 2012,Accepted 21st October 2012
DOI: 10.1039/c2ra20083j
www.rsc.org/advances
Rick F. Rajter,a Roger H. French,b W.Y. Ching,c Rudolf Podgornikde and V.Adrian Parsegian*f
Optical dispersion spectra at energies up to 30 eV play a vital role in understanding the chirality-
dependent van der Waals–London dispersion interactions of single wall carbon nanotubes (SWCNTs). We
use one-electron theory based calculations to obtain the band structures and the frequency dependent
dielectric response function from 0–30 eV for 64 SWCNTs differing in radius, electronic structure
classification, and geometry. The resulting optical dispersion properties can be categorized over three
distinct energy intervals (M, p, and s, respectively representing 0–0.1, 0.1–5, and 5–30 eV regions) and over
radii above or below the zone-folding limit of 0.7 nm. While p peaks vary systematically with radius for a
given electronic structure type, s peaks are independent of tube radius above the zone folding limit and
depend entirely on SWCNT geometry. We also observe the so-called metal paradox, where a SWCNT has a
metallic band structure and continuous density of states through the Fermi level but still behaves optically
like a material with a large optical band gap between M and p regions. This paradox appears to be unique
to armchair and large diameter zigzag nanotubes. Based on these calculated one-electron dielectric
response functions we compute and review van der Waals–London dispersion spectra, full spectral
Hamaker coefficients, and van der Waals–London dispersion interaction energies for all calculated
frequency dependent dielectric response functions. Our results are categorized using a new optical
dielectric function classification scheme that groups the nanotubes according to observable trends and
notable features (e.g. the metal paradox) in the 0–30 eV part of the optical dispersion spectra. While the
trends in these spectra begin to break down at the zone folding diameter limit, the trends in the related
van der Waals–London dispersion spectra tend to remain stable all the way down to the smallest single
wall carbon nanotubes in a given class.
1 Introduction
Since their discovery in 1993 by the Iijima and the Bethunegroups,1,2 single wall carbon nanotubes (SWCNTs) havereceived enthusiastic attention. Their intriguing mechanicaland electrical properties make them ideal for a wide range ofapplications, from metal oxide semiconductor field effect
transistors (MOSFETs) to novel drug delivery systems3–8 andhave inspired strong scientific and industrial interest.1,9–15
The area that has arguably received the most attention andfocus is their electronic structure and characterization.16–19
The reason is that SWCNTs are a unique class of materials inwhich small changes in their atomic structure and geometrycharacteristics (quantified by the chirality vector (n,m) orequivalently by [n,m, type], when we want to stress the type ofthe nanotube3) determines whether they behave as a dielectric,a metallic conductor or a semiconductor. They are also very
aDepartment of Materials Science and Engineering, Massachusetts Institute of
Technology, Cambridge, Massachusetts 02139-4307, USAbDepartment of Materials Science and Engineering, Case School of Engineering, Case
Western Reserve University, Cleveland Ohio, 44106-7204, USAcDepartment of Physics and Astronomy, University of Missouri-Kansas City, Kansas
City, Missouri, 64110, USAdDepartment of Physics, Faculty of Mathematics and Physics, University of Ljubljana,
1000 Ljubljana, SloveniaeDepartment of Theoretical Physics, J. Stefan Institute, 1000 Ljubljana, SloveniafDepartment of Physics, University of Massachusetts, Amherst MA 01003, USA.
E-mail: [email protected]
3 In the context of the dielectric response functions of CNTs, we denote theSWCNT with a mnemonic [n,m, type] rather then the standard but equivalent(n,m), when we want to invoke its type explicitly in order to help the readerorganize the voluminous information and in order to be consistent with ourprevious publications. Of course the two designations, together with the simple(n 2 m)/3 = integer rule to identify the metallic and semiconducting nanotubes,9
are equivalent.
RSC Advances
PAPER
This journal is � The Royal Society of Chemistry 2013 RSC Adv., 2013, 3, 823–842 | 823
narrow (typically ¡1 nm wide) and inexpensive to produce,making them ideally suited for many nano-electronic applica-tions although widespread commercial and industrial use hasyet to be achieved. While there has been some recent progressin the purification of SWCNTs from residual amorphouscarbon or bundled SWCNTs, that sometimes also leads todiameter-selective separation of SWCNTs,20 it is in general stilldifficult to place them into predetermined arrangements.21–25
Solving the assembly problem, which has been addressed onvarious levels beginning shortly after the discovery of CNTs,26
represents an important next step based on the detailedmolecular structure of various SWCNTs that determines theiroptical properties and through them their interactions: asubject of this review.
Understanding the optical dispersion properties ofSWCNTs is crucial to their role in several long-rangeinteractions, especially the van der Waals–London dispersion(vdW–Ld) interaction. Each SWCNT is uniquely defined by itschirality vector (n,m), which denotes the circumferentialwrapping direction along a graphene sheet containing sp2
hybridized carbon bonds.9,17,27 Thus, each (n,m) combinationdenotes a different geometrical construction that is respon-sible for the wide variety of electronic structure, phonon, andRaman behavior.28–30 The same diversity that makes themappealing also for performance leads to selectivity andspecificity in sorting and placement. This is seen in AC/DCexperiments,31 dielectrophoresis,32 and anion IEC.23–25 Eachchirality vector gives SWCNTs a unique set of properties (e.g.,band gap, van Hove singularities (vHs), etc.), but theircommon composition and chemical bonding coupled withsymmetry considerations makes it possible to categorize themby their particular features.27,30
A comprehensive study of CNT interactions can provide thefundamental conceptual framework required for proper under-standing of experiments on their separation, placement andassembly. Among these interactions, the universal and longestrange, the van der Waals–London dispersion (vdW–Ld) inter-action, merits most detailed scrutiny. First, because theseinteractions are long range and ever-present in nature, alwayscontributing to and influencing the overall interaction betweencharge-neutral bodies,33 second, previous results34–36 show thatthe magnitude of this interaction for various CNTs can vary by20% even in simple systems, making it a convenient candidateto control experimentally, and third, SWCNTs have well knowntrends in their electronic structures as a function of chirality,19
which could then act as the source for chirality-specific vdW–Ldinteractions.
During the last few years it has become possible to computequantitative direction-dependent optical dispersion proper-ties, such as the frequency-dependent complex dielectricfunction e vð Þ~e0 vð Þzie’’ vð Þ, for a diverse set of isolatedSWCNTs, for which spectroscopic techniques even as powerfulas electron energy loss spectroscopy (EELS),37,38 which requiresbulk sample of identical SWCNTs in a bundle,39 cannot be applieddirectly. The use of one-electron theory based calculations allowsus to circumvent these shortcomings but still use available
experimental results to compare and confirm the integrity of ourspectral data.40–42 We were able to resolve the axial and radialdirection of SWCNTs to obtain the optical dispersion propertiesout to photon energies of at least 30 eV. Also, we were not limitedto the SWCNTs that are easily produced by existing preparationmethods,43,44 which allowed us to study a larger set of data thanwould otherwise be possible.
Early attempts to obtain this information via ab initio codesproduced unreliable results above 20 eV and were limited to asingle nanotube.41 Some computational studies were able toinvestigate a large quantity of chiralities, but they wereconfined to dispersion properties below 6 eV because theyrelied on the tight binding approximation, which artificiallydistorts the bands.45 New ab initio results are emerging thathave accurate dispersion properties along the entire interval,but continue to be confined to a select number of chiral-ities.40,42 Here we calculate and review the optical dispersionproperties, represented as the imaginary part of the dielectricresponse function, e99(v), up to 30 eV for 64 SWCNTs that havevarying diameter, electronic structure classification, andgeometry. We follow trends and variations to give insight forsystem design. Later, we use these dielectric responsefunctions to analyze consequences of different spectralproperties in vdW–Ld interaction energies.
Trends and deviations from these trends in SWCNT opticaldispersion spectra are categorized into a new SWCNTclassification scheme, based on a combination of electronicstructure, geometry and curvature. The links between chirality,cuttings lines, band diagrams, density of states and opticaldispersion properties are extended to the magnitude of vdW–Ld interaction as quantified by the Hamaker coefficients forchirality-dependent vdW–Ld interactions. We highlight the keyremaining features linking the dielectric function e99(v), withthe consequent vdW–Ld interaction energy.
2 Electronic structure and optical dispersionspectra
2.1 Method
The method for calculation of the electronic structure andoptical properties is the first principles orthogonalized linearcombination of atomic orbital (OLCAO) method which isdescribed in detail in ref. 46. The OLCAO method is applied tothe calculation of the electronic structure and optical disper-sion spectra of 64 SWCNTs. It yields the imaginary part of thefrequency-dependent dielectric response function, e99(v),calculated within the random phase approximation (RPA) ofthe one-electron theory.47 The optical transitions from thevalence band (VB) to the conduction band (CB) are calculatedfrom the ab initio wave functions using the extended basis(EB). The ab initio nature of the wave function ensures thestrict adherence of the selection rules via the momentummatrix elements. If an optical transition is symmetry for-bidden, it automatically has a zero momentum matrix and notransition will occur even if such a transition appears to beavailable via the density of states (DOS). A key example that we
824 | RSC Adv., 2013, 3, 823–842 This journal is � The Royal Society of Chemistry 2013
Paper RSC Advances
will show later is when a SWCNT’s DOS has a continuousseries of states across the Fermi level and yet behaves like asemiconductor with no transitions below 1 eV. All the relevantdetails of the calculation have been described in ref. 34, 35 and48.
Though not taken into account by the one-electron method,we are fully aware of the importance of the excitoniceffects49,50 in the low dimensional systems such as grapheneand CNTs.51–65 They tend to introduce additional peaks in theenergy range below 5 eV or slightly shift the position of someother peaks. From a pure theoretical point of view, the effect ofexcitons has been intensively studied and can be approachedfrom many different angles including two-photon excitation,excitons of delocalized higher levels etc. An importantquestion in this respect is to what extent the excitonic peakscan modify the optical absorption obtained from the one-electron theory? In some cases the traditional one-electroncalculation of optical properties gives dielectric constants orthe refractive indices in good agreement with experiments onmany insulating materials. However, though the excitoniceffects in the case of SWCNT optical spectra are important andeminently measurable,28,29 it is nevertheless not clear how thechanges in optical spectra due to excitonic effects will affect theoverall Hamaker coefficients and the trends in the vdW–Ldinteraction between different classes of SWCNTs. Since thevdW–Ld interaction is a functional (or more precisely adiscrete sum over the Matsubara frequencies) of the fre-quency-dependent dielectric response, it is reasonable toexpect that such effects will be small and that the strengthof the interaction will depend more on the global properties ofthe dielectric response delimited by the sum rule than on localspecifics. (see later results in section 6.3).
The above conjecture is supported by the recent work ofHobbie and co-workers on empirical evaluation of attractivevdW potential in SWCNTs.66 Even though they have alsorecognized the presence of excitonic effect in CNTs, theauthors used a much simpler empirical approach by fitting thecollective peaks to a superposition of individual Lorentzians.They have concluded that for the semiconducting nanotubes,neglecting the three optical resonances reduces the Hamakercoefficient by roughly 5%, while neglecting the Drude termdecreases the Hamaker coefficient by roughly 2%. For themetallic SWCNTs, neglect of either of these terms reduces theHamaker coefficient by roughly 3%. In this view, excitoniceffects certainly have a small but measurable effect and alarger question is now how they influence the plasmons. Fromthe ab initio perspective, a first-principles approach thatcorrectly accounts for electron-hole interactions in quasi-1Dsystems would thus provide a more accurate computationalfoundation, but only to the extent that it also accuratelydescribes the two plasmons. On the other hand, practicalapplications to real problems using optical spectra obtainedfrom one-electron calculation is an attractive alternative asindicated in another recent paper on adhesion in siliconwafers.67
The fundamental theory of the calculation method withinthe framework of the DFT is sound. Although many-bodyinteractions are not considered and there may be concernsabout the underestimation of the band gap, they are less
important in this study since our main focus is on the vdW–Ldspectra of a large number of CNTs up to high frequency andtheir systematic correlations to the structure. In contrast, inthe tight binding approximation (TBA) method where noaccurate wave functions are involved, the band gaps aretypically adjusted in order to best describe and represent thestates very near the band gap. States several eV beyond theband gap are ignored or poorly represented.45 In addition, TBAmodels would not be able to predict novel departures from themain SWCNT structural trends. There are several examples ofthis, such as 1) the [5,0,s] actually is a metallic conductorinstead of being semiconductor-like,45 and 2) the [6,0,m] has alarge degree of hybridization of graphene sp2 and p bonds intosp3 bonds and thus a band diagram unlike any other armchairSWCNT.30 Ab initio codes capture these major departures fromthe trends without requiring ipso facto arbitrary adjustments.On the other hand, inclusion of excitonic corrections based onmany-body theory is not feasible in the OLCAO method whichuses local atomic orbitals for basis expansion rather thanplane waves. It is interesting to note that empirical TBA canalso be refined to investigate the excitonic effect in SWCNT ashas been demonstrated by the work of Jiang et al.63
The OLCAO method is an all-electron method with aneconomical use of the basis expansion. The full secularequation is diagonalized to obtain all electron states includinghigh energy CB states. If an iterative procedure is used for theelectron states, only a small number of CB state wavefunctions are usually obtained. To obtain higher energy CBstates in an iterative approach for systems with a large numberof atoms in the unit cell could be computationally prohibitive.The dipole matrix elements of transitions between the VB andCB are accurately calculated from the ab initio wave functionsand explicitly included in the optical dispersion spectracalculation, which automatically imposes the selection rulesfor the transition.
The OLCAO method is versatile and can be applied toalmost any material whether it is a metal or an insulator, aliquid or an amorphous solid, an inorganic crystal or abiomolecule, having an open structure or a compact one, orwhether it contains light elements (such as H or Li) or heavyatoms (such as rare earth elements). The method avoids theuse of atomic radii in the calculation, which could beproblematic for complex materials with different local bond-ing. Finally, the use of local atomic orbitals facilitates theinterpretation of the physical properties where p or s statesplay a crucial role in the optical spectra of SWCNTs. Theefficient evaluation of multicenter integrals in analytic formsmakes the method highly efficient and eventually applicable tolarge complex systems such as DNA molecules in a fluidmedium. For example, application to the calculation of largeanisotropic optical absorption in herapathite crystal((C20H24N2O2H2)4 6 C2H4O2 6 3SO4 6 2I3 6 6H2O), acomplex multi-component organic crystal with 988 atoms inthe unit cell yields excellent agreement with the measureddata.68 Application of the OLCAO method to the spectroscopicproperties of a large model of super-cooled water is equallysuccessful.69
This journal is � The Royal Society of Chemistry 2013 RSC Adv., 2013, 3, 823–842 | 825
RSC Advances Paper
2.2 Case study: SWCNT: [7,5,s] vs. [8,2,m]
Each SWCNT chirality (n,m) defines a unique geometricalconstruction that results in a distinct set of electronic andoptical dispersion properties. Because of their similarity tographene in composition and structure, there are somefeatures common among all SWCNTs, however, there are alsotwo fundamental differences: circumferential periodicity andcurvature. Periodicity along the circumference allows onlydiscrete lines of states out of the continuum available forgraphene, while curvature placed upon a flat graphene sheetre-hybridizes the sp2 lattice to include sp3 like states.19
For an infinite diameter SWCNT, the number of availablestates is a continuum equivalent to nearly flat sp2 sheets ofgraphene. The only differentiating feature among variousinfinite diameter tubes would be the bonding direction alongthe axial direction. For a large, but finite diameter SWCNT, theeffects of periodicity would cause a set of discrete allowablestates in the axial direction. However, because the carbonbonds would still be relatively flat (i.e., still nearly perfect sp2
bonds), it is possible to derive a SWCNT’s band structure byselecting the allowable states from the band diagram ofgraphene. Such an approximation is called the zone-folding
approximation; it is valid only for SWCNTs of diameter greaterthan 1 nm. Below this threshold, the curvature of the SWCNTwall becomes so pronounced that the bonds gain a significantsp3 characteristic. For very small tubes, using a zone foldingprocedure can be problematic.19,30,45,70
Each SWCNT chirality represents a unique geometricalconstruction of a 1D tube of sp2 carbon bonds created from arolled up sheet of graphene. What makes SWCNTs such ahighly studied set of materials is the number of materialproperties that significantly change as a function of chirality.Perhaps the best well known is metallic versus semiconductingbehavior, depending whether or not (n 2 m)/3 is an integer.Variations in properties propagate through several features,for example: linkages between chirality, cutting lines, banddiagrams, density of states, optical dispersion properties,Hamaker coefficients, extending to chirality-dependent vdW–Ld interactions. Fig. 1 shows these differences for the metallic[8,2,m] and the semiconducting [7,5,s].
While some of these relationships (e.g., chirality to electro-nic band diagram) have been extensively studied and somepredictive rules are widely used, much information at theoptical level cannot be easily predicted a priori or explained
Fig. 1 Layers of abstraction of SWCNT properties ranging from [n,m] to the optical dispersion spectrum e99(v) for the [7,5,s] semiconductor and [8,2,m] metal. (a) Thegeometrical construction. (b) A chirality map showing all 5 types of SWCNT. (c) The cutting lines across the Brillouin zones for two different types of SWCNT, [7,5,s]and [8,2,m], within the dispersion classification. The dot represents the K point in the Brillouin zone. (d) The optical dispersion spectrum e99(v) in both the radial andaxial direction. Frequency in eV.
826 | RSC Adv., 2013, 3, 823–842 This journal is � The Royal Society of Chemistry 2013
Paper RSC Advances
Table 1 Tabulated data of all SWCNTs. The chirality vector (n,m) determines the radius, angle, and geometry. The classification depends on the relationship between(n,m) and symmetry. The number of atoms required for a lattice repeat in the ab initio calculations is also included
n{m3
sp2–sp3 Symmetryn m Radius (Å) Angle Geometry Zone folding Lambin Saito Atoms
3 3 2.034 30.00 armchair metal metal M-2p 124 4 2.712 30.00 armchair metal metal M-2p 165 5 3.390 30.00 armchair metal metal M-2p 206 6 4.068 30.00 armchair metal metal M-2p 247 7 4.746 30.00 armchair metal metal M-2p 288 8 5.424 30.00 armchair metal metal M-2p 329 9 6.102 30.00 armchair metal metal M-2p 36
10 10 6.780 30.00 armchair metal metal M-2p 4011 11 7.458 30.00 armchair metal metal M-2p 4412 12 8.136 30.00 armchair metal metal M-2p 4813 13 8.814 30.00 armchair metal metal M-2p 5214 14 9.492 30.00 armchair metal metal M-2p 5615 15 10.170 30.00 armchair metal metal M-2p 6016 16 10.848 30.00 armchair metal metal M-2p 6417 17 11.526 30.00 armchair metal metal M-2p 6818 18 12.204 30.00 armchair metal metal M-2p 7219 19 12.882 30.00 armchair metal metal M-2p 7620 20 13.560 30.00 armchair metal metal M-2p 8021 21 14.238 30.00 armchair metal metal M-2p 8422 22 14.916 30.00 armchair metal metal M-2p 8823 23 15.594 30.00 armchair metal metal M-2p 9224 24 16.272 30.00 armchair metal metal M-2p 96
6 0 2.349 0.00 zigzag metal semimetal M1 249 0 3.523 0.00 zigzag metal semimetal M1 36
12 0 4.697 0.00 zigzag metal semimetal M1 4815 0 5.872 0.00 zigzag metal semimetal M1 6018 0 7.046 0.00 zigzag metal semimetal M1 7221 0 8.220 0.00 zigzag metal semimetal M1 8424 0 9.395 0.00 zigzag metal semimetal M1 9627 0 10.569 0.00 zigzag metal semimetal M1 10830 0 11.743 0.00 zigzag metal semimetal M1 120
7 0 2.740 0.00 zigzag semi semiconductor S1 288 0 3.132 0.00 zigzag semi semiconductor S2 32
10 0 3.914 0.00 zigzag semi semiconductor S1 4011 0 4.306 0.00 zigzag semi semiconductor S2 4413 0 5.089 0.00 zigzag semi semiconductor S1 5214 0 5.480 0.00 zigzag semi semiconductor S2 5616 0 6.263 0.00 zigzag semi semiconductor S1 6417 0 6.655 0.00 zigzag semi semiconductor S2 6819 0 7.437 0.00 zigzag semi semiconductor S1 7620 0 7.829 0.00 zigzag semi semiconductor S2 8022 0 8.612 0.00 zigzag semi semiconductor S1 8823 0 9.003 0.00 zigzag semi semiconductor S2 9225 0 9.786 0.00 zigzag semi semiconductor S1 10026 0 10.178 0.00 zigzag semi semiconductor S2 10428 0 10.960 0.00 zigzag semi semiconductor S1 11229 0 11.352 0.00 zigzag semi semiconductor S2 116
5 2 2.445 16.10 chiral metal semimetal M-2m 526 3 3.107 19.11 chiral metal semimetal M1 847 4 3.775 21.05 chiral metal semimetal M-2p 1248 2 3.588 10.89 chiral metal semimetal M-2p 568 5 4.446 22.41 chiral metal semimetal M-2m 1729 3 4.234 13.90 chiral metal semimetal M1 156
10 4 4.889 16.10 chiral metal semimetal M-2m 10411 2 4.746 8.21 chiral metal semimetal M-2m 19611 8 6.468 24.79 chiral metal semimetal M-2m 364
4 2 2.071 19.11 chiral semi semiconductor S2 565 1 2.179 8.95 chiral semi semiconductor S1 1246 1 2.567 79 chiral semi semiconductor S2 1726 2 2.823 13.90 chiral semi semiconductor S1 1046 4 3.413 23.41 chiral semi semiconductor S2 1526 5 3.734 27.00 chiral semi semiconductor S1 3647 5 4.087 24.50 chiral semi semiconductor S2 4369 1 3.734 5.21 chiral semi semiconductor S2 364
This journal is � The Royal Society of Chemistry 2013 RSC Adv., 2013, 3, 823–842 | 827
RSC Advances Paper
simply by knowing (n,m). Perhaps the most notable example isbetween the electronic structure and optical levels, whichexhibit many non-linear relationships and other features thatoffer somewhat surprising results. The need is to determinethe optical dispersion properties for most chiralities ratherthan approximate/derive them from a SWCNT of seeminglysimilar characteristics.
The introduction of ab initio e99(v) optical dispersionproperties enables such an analysis, which would be verydifficult experimentally. Fortunately, the experimental datathat do exist (notably the EELS data by Stephan et al.37)compare favorably to our results. Although they specify tubesby diameter and not chirality, they do note major peaks thatappear consistently across tubes of all diameters. Mostnotably, their results show three major peak areas: bandgap, transitions at 4 eV, and transitions at 15 eV. There are alsolow flat areas between 5–12 eV and beyond 20 eV. These resultsare in qualitative agreement with our [7,5,s] and [8,2,m] abinitio optical dispersion properties. The only major differenceappears to be in the balance of the e99(v) peak heights andtotal areas within the p and s regions. However, thesedifferences may resolve when experimental data can be morereadily divided into the radial and axial components, orperhaps a finer experimental energy resolution would help.
2.3 SWCNT classification schemes
Table 1 lists the 64 SWCNTs studied here, with their figures ofmerit (n, m, radius, angle, geometry, and number of atoms perlattice repeat), and the three classification schemes (zonefolding, Lambin,19 and Saito9). Our proposed dispersionclassification (not in Table 1) is essentially a combination ofthe Lambin and geometrical descriptors. Although thistechnically leads to nine possible combinations, only five ofthem are allowed for smaller diameter SWCNTs. For instance,an armchair SWCNT’s electronic structure is never semicon-ducting unless there are added defects, functional groups, orother influential external sources such as a strong externalfield.71–74 For the larger-diameter limit, the divisions maybecome redundant as the semimetal gap becomes so small(i.e., less than 0.01 eV) that it essentially blurs the line of themetal/semimetal division.
Fig. 1 shows the cutting lines for the SWCNTs representingan example of two types of the dispersion classification, [7,5,s]and [8,2,m]. It is the relationship of cutting line angle,location, and density that determines if and when the cuttinglines cross/graze the K points at the edge of the BZ and resultin a metal/semimetal electronic structure. Nanotubes of verydifferent cutting line density and angle (i.e., the [6,5,s] and the[9,1,s]) can have different cutting line angles and yet similarband gaps. Conversely, tubes that appear to have very similarcutting line angles and density (i.e., the [9,0,m] versus the[10,0,s]) fall into different classifications altogether. Such isthe delicate nature of the electronic structures dependence on(n,m). The cutting line representation in the BZ has served asthe basis for every major SWCNT classification thus far (i.e.,simple, Lambin, and Saito). In the zone-folding classification,the effects of curvature on the carbon sp2 bonds are ignoredand the only thing that differentiates the basic metallic andsemiconducting classifications is whether a K point is crossed.
This results in the simple (n 2 m)/3 = integer rule.9 TheLambin system acknowledges the changes in sp2 bond anglesand lengths as a result of the cylindrical nature ofSWCNTs.19,30 This curvature causes a slight distortion in thestructure and the resulting BZ contains cutting lines thatbarely miss or graze the K-points and don’t directly crossingthem. This opens up the tiniest of band gaps (ranging from0.02 to 0.05 eV) for tubes that the zone-folding classificationwould predict as perfect metals with no band gaps. Fig. 2illustrates the cutting line diagrams and resulting electronicband structures of these three types. The [9,3,m] has a barelyvisible 0.02 eV band gap. For comparison, the Lambin modelpredicts a gap of approximately 0.07 eV.
Fig. 2 A comparison of the band diagrams and cutting lines for three SWCNTsrepresenting the Lambin classification system. Note the subtle differencebetween the [6,6,m] and the [9,3,m]. The [6,6,m] has no band gap whereas the[9,3,m] has CB and VB just miss touching. Thus the [9,3,m] is actually a smallband gap semiconductor.
828 | RSC Adv., 2013, 3, 823–842 This journal is � The Royal Society of Chemistry 2013
Paper RSC Advances
Finally, the Saito method9 returns to the zone-foldingscheme (i.e., ignores the effects of the structural relaxation),but it considers additional symmetry effects that can furtherdifferentiate tubes into numerous groupings.9 For example,the semiconductors can be subdivided into two classes basedon the relationships of the first cutting line’s position relativeto the K point. Neither the proposed dispersion classificationnor the available classifications can adequately predict thedispersion properties of the smallest SWCNTs. At this limit,there is a strong reintroduction of sp3-like bonding, which canengender new bands within the electronic structure as well assignificantly shift other features. For this reason, [5,0,s] ismetallic despite no classification predicting it.45 It appears,however, that there are very few of these exceptions. Therefore,one should always seek additional experimental or ab initioconfirmation when describing the dispersion properties ofvery small SWCNTs.
2.4 Influence of structural parameters on optical transitions
Despite the shortcomings in each of the given classifications,they are powerful tools that can help to map out andunderstand global trends. The first trend is that the packingdensity of cutting lines varies systematically as a function ofradius, creating a diameter-dependent band gap and trends inthe axial e99(v) peaks. Fig. 3 shows e99(v) for three differentarmchair SWCNTs, [4,4,m], [14,14,m] and [24,24,m].Increasing the SWCNT radius allows more lattice translationsin the circumferential direction and thus a larger degree ofcutting line packing. Dresselhaus and Saito quantified thedensity of cutting9,28 and showed that this increase in thecutting line density means that the cutting line closest to the Kpoint will push closer to it. Therefore, the larger the SWCNTradius, the larger its cutting line density and the smaller thedifference between its first conduction and valence bands.This causes a systematic shift in the DOS and e99(v) peaks tolower energy (a well known effect).27,28,30 Additionally, itmeans that larger tubes will have more of these peaks becauseof an increased availability of cutting line transitions. Note
that these shifts of e99(v) peak position as a function ofdiameter are only valid for the axial direction p peaks. In Fig. 3(a), one can see that all the SWCNTs have a final e99(v) peak(the p0 peak) at 4.20 eV in the p transition region. This is dueto the cutting lines reaching some common border for allarmchair SWCNTs. All peaks beyond this 4.20 eV p0 peak, inthe 5–30 eV s transition region in Fig. 3 (b) are invariant withchange in radius.
Before investigating the differences in these two regimes, wefirst considered the known variation in e99(v) peak locationsbetween the metal and semiconductor classifications in the p
regime. When a K point is crossed, the next nearest cuttingline is a full spacing away. Conversely, the semiconductingtubes have their first two cutting lines at 1/3 and 2/3 of thisdistance. The implications of this are: metals cross a K-pointwhere the CB and VB meet, allowing for the possibility of afinite-height metal peak all the way down to 0.00 eV. Symmetryeffects are the only thing that prevent it from appearing in thee99(v) optical dispersion properties. Additionally, metals havetheir next nearest cutting line at an energy three times largerthan that of a semiconductor of equivalent radius. Therefore,while the p peaks in e99(v) from 0–4 eV will shift systematicallyas a function of radius for tubes of similar electronic structure(i.e., metals or semiconductors), there is a big shift in the peaklocations between the classifications.9,30
As seen in Fig. 3 (b), the s transitions seen in the 5–30 eVoptical dispersion properties seem to be invariant with respectto changes of CNT radius. But are the data in this regime thesame for all SWCNTs or is there another parameter that canmake a difference? If we compare a zigzag semimetal with azigzag semiconductor, we have essentially fixed the geometryand tested whether there is a correlation with the electronicstructure properties of the p regime. Likewise, if we comparezigzag semimetals with armchair metals, we have essentiallyfixed the electronic structure while varying thegeometry.{Comparing all three would allow us to check ifthere is a simultaneous correlation with both geometry and 0–5 eV electronic structure. Fig. 3 (a) and (b) combined with
Fig. 3 The axial component of the optical dispersion spectrum e99(v). (a) e99(v) in the 0–5 eV region. (b) e99(v) in the 0–30 eV region, both for the case of [18,18,m],[21,21,m] and [24,24,m] SWCNTs. Note that as the cutting line density increases for larger tubes, there is a systematic shift of the first e99(v) p1 peak towards 0 eV.However, the optical dispersion spectrum e99(v) above 5 eV appears to be largely invariant with respect to changes in diameter for large tubes. Frequency in eV.
This journal is � The Royal Society of Chemistry 2013 RSC Adv., 2013, 3, 823–842 | 829
RSC Advances Paper
Fig. 4 (a) and (b) show just such a comparison of the threeSWCNT types for both the 0–5 and 5–30 eV ranges. The p
regime behaves as expected with its dependencies on radiusand zone-folding classification. The e99(v) peaks of themetallic and semiconducting zigzag SWCNTs are visuallyidentical in the s regime, eliminating any correlation to thezone-folding classification. However, there is a clear differencein e99(v) peak magnitude and position between the armchairand zigzag geometries, suggesting geometry as the influentialparameter in the s regime.
3 Features and analysis of spectralproperties
Because we have observed trends in spectral properties for thelargest diameter SWCNTs (i.e., in the zone folding regime), it isinstructive to ask how resilient they are. Do they work down tothe smallest radius SWCNTs? Is there a particular cutoff forthe range/diameter? Are the departures from the trends subtleor are they large, leading to a seemingly random set ofproperties among the chiralities? Fig. 5 (a) to (d) shows e99(v)peak position vs. radius for the armchair SWCNTs from [3,3,m]to [24,24,m] in both axial and radial directions in two energyranges separated at the critical radius of 0.7 nm. In the 0–5 eVrange there is a smooth trend down to the tiniest of SWCNTs.However, in the s regime, we see a large distortion of peaks forradii of less than 0.7 nm. New peaks appear to form and othersappear to shift randomly.§
In the case of SWCNTs we detect additional p–s* and s–p*-like transitions due to curvature causing these otherwiseindependent directions to overlap. As a result, between thelimit of 3.8 eV (all p–p* transitions below) and 10.0 eV
(significant s–s* transitions above), it is not clear whichparticular transitions contribute most to the optical dispersionproperties. The goal here, however, is simply to categorize thetwo distinctly different regimes found in Fig. 4 and 5.Ultimately our selection of 5 eV as the p/s cutoff was basedon three major factors: 1) Large diameter SWCNTs typicallyhave no major e99(v) contributions between 5–10 eV for theaxial and/or radial directions. Thus we could arbitrarily selectany location along this interval without changing around thedistributions of peaks contained in each of the groups. 2)Since the edge between p–p* and non p–p* related e99(v)contributions is the only hard edge known with certainty, itmakes sense to select the lowest energy in the 5–10 eV interval.Therefore, our p classification for SWCNTs is purely p–p*based while anything above 5 eV is likely to have contributionsfrom all 4 possibilities (p–p*, s–p*, p–s*, and s–s*). 3) InFig. 5, the smallest SWCNTs have the largest curvature andtherefore the highest degree of p–s* and s–p* overlap. This islikely the reason for the increase in e99(v) peaks appearing inthe 5–10 eV limit.
3.1 Metal peak analysis
An ideal metal is characterized by a simple Drude modelcorresponding to
e’’ vð Þ~ 4pNe2
m|
t
v(1zt2v2)~v2
p
t
v(1zt2v2)(1)
where N is the electron density, m the electron mass, and vp
the characteristic plasma frequency. This expresses thedivergence of the dielectric response at vanishing frequencies.This feature, while not critical to our studies of SWCNTs, is atopic of interest in the formulation of electrodynamic forcesdue to the importance of conductivity effects.75–78 In computa-tion, we can only approach the static limit asymptotically.
Fig. 4 Comparison of e99(v) optical dispersion spectrum in the (a) p (0–5 eV) and (b) s (5–30 eV) regions along the axial direction for metallic and semiconductingzigzag SWCNTs. Frequency in eV.
{ Technically, semimetals and metals have differences in their properties at theFermi level. However, we are more interested in whether the relationships of thecutting lines with the K-points also impact the 5–30 eV properties in anysignificant way, making the crossing/grazing differentiation irrelevant.
§ Note that a change in quantity of peaks doesn’t necessarily change the overallmagnitude. It simply is a useful parameter to monitor when studying changesamong the various chiralities.
830 | RSC Adv., 2013, 3, 823–842 This journal is � The Royal Society of Chemistry 2013
Paper RSC Advances
In computation we can distinguish three types of behaviorin this metallic peak energy range. We refer to these behaviorsas null, M0, and M1. Null represents a SWCNT with at least a0.1 eV optical band gap. For a M0 peak, e99(v) risesasymptotically as the energy approaches 0 eV, while a M1
peak will rise in a similar manner but then falls back to a valueof e99(v) = 0 at an energy in the range from 0.02 to 0.05 eV. Itshould be noted that very small band gaps (less than 0.05 eV)do exist in materials and in this work the M1 type metal peaksare not likely due to a computational artifact since we calculatethe optical transitions and dipole matrix elements down to0.01 eV transition energy.
Consider the optical dispersion properties of three SWCNTsrepresenting the armchair metal, zigzag metal, and chiralmetal classes. In a zone-folding classification, these would allbe considered metals and therefore the 0 eV behavior shouldbe indistinguishable for all three cases. The Lambin classifica-tion would state that the [9,9,m] armchair is a true metal, butthe [18,0,m] and [9,3,m] would experience a slight gap of lessthan 0.1 eV. Therefore we would expect to potentially see twotypes of behavior at 0 eV. In actuality, we see all three metalbehaviors: null (armchair), M1 (chiral metal), and M0 (zigzagmetal). The most surprising observation is that of the [9,9,m]armchair. Despite having no band gap and a tiny butcontinuous DOS around the Fermi level, it exhibits no opticaltransitions from 0 to 1.5 eV. This effect is somewhat
paradoxical because the armchair SWCNTs represent the onlyclass with no band gap (not even a very small band gap like thezigzag and chiral semi-metals), and yet they exhibit opticalband gaps as large as 1 eV. Also unexpected is the M0 peak ofthe [18,0,m] because zigzag metals are supposed to have a verysmall, but finite band gap, and thus we would expect an M1
type peak. Perhaps structural relaxation would resolve thisinconsistency and uncover an M1 type peak instead.19 If,however, this proves to be a real and accurate result, thendividing the metals into these three metal categories isjustified because it will result in three types of vdW–Ldinteractions.
Because physical properties depend strongly on the exis-tence and magnitude of an M0 or M1 peak, we wanted todetermine if such peaks scale with SWCNT radius. Fig. 6 (a)compares the e99(v) dispersion properties in the 0–1.5 eV rangeacross 8 different zigzag metal SWCNTs. There is a clearlyinverse relationship between the metal peak magnitude andradius with the [9,0,m] having a M0 peak of approximately20 000. This magnitude systematically diminishes until[24,0,m], where the M0 peak opens up to a very weak M1 peak.For larger tubes, this peak disappears altogether.
Do chiral metals experience a similar M0/M1 trend as afunction of radius? Not according to the metal peaks for thenine chiral metal SWCNTs listed in Table 1. The largest M0
peaks come from the [5,2,m] and the [10,4,m] SWCNTs, which
Fig. 5 Plots of peaks in optical dispersion spectrum e99(v) vs. the radius of SWCNTs. (a) Axial direction from 0–5 eV in the p region. Smooth trends observed for all radii;(b) radial direction from 10–20 eV in the s region. No trends for small radius tubes; (c) axial direction from 0–5 eV in the p region. Smooth trends observed for all radii;and (d) radial direction from 10–20 eV. No trends for small radius tubes. Frequency in eV.
This journal is � The Royal Society of Chemistry 2013 RSC Adv., 2013, 3, 823–842 | 831
RSC Advances Paper
respectively have the smallest and second largest radius withinthe group. The other seven chiral metals have M1 and M0
peaks that are weaker by 1 to 2 orders of magnitude. Morelarge-diameter chiral metals are need to be studied, but theyare more difficult to study as they often require up to an orderof magnitude more atoms within the unit cell of the ab initiocalculation.
A Drude metal shows a 1/v divergence of the dielectricresponse function (eqn (1)), giving a slope of 21 in a log-logplot of e99(v). Fig. 6 (b) shows this plot for five zigzag metallicSWCNTs. Instead of observing a slope of 21 (not shown), weobserve a slope of 22. The significance of this difference is notclear.
3.2 p and s region analysis
All large diameter SWCNTs show a p0 peak in e99(v) at 4.0–4.3eV that is invariant with respect to changes in radius for agiven SWCNT class and direction (i.e. radial or axial). Forarmchair SWCNTs [see Fig. 3 (a) and (b)] the p0 peaks occur at4.19 eV and 4.21 eV for the axial and radial directions,respectively. However, for armchair tubes with diametersbelow the zone-folding limit, these peaks shift noticeably withthe axial (radial) direction shifts slightly lower (higher) as afunction of 1/radius. Why these peaks are pinned at the largediameter limit and shift in opposite directions at the smalldiameter limit is unclear. It is conceivable that all SWCNTsexperience some common edge in the BZ that begins todissolve as the cutting line density decreases and the bonddistortion increases.
The next important peak is associated with the optical bandgap, labeled p1. All other peaks between p1 and p0 areincrementally labeled p2, p3, etc., if they exist [see Fig. 3 (b)].The largest SWCNTs in this study have up to six p peaks in theaxial direction. The radial direction typically has only p0 and p1
peaks with relatively flat, low regions in between.Zigzag metals and semiconductors have a little more
variation in their p0 peaks as shown in Fig. 4 (a) and Fig. 4(b). The values typically oscillate between 4.00 and 4.30 for thelargest zigzag SWCNTs in the axial direction, with the variation
increasing versus 1/radius. Just like the armchair SWCNTs, thepeaks in the radial and the axial directions shift in theopposite direction as the radius decreases. The p0 peaks forchiral metals and semiconductors are a bit varied. We have nodata for SWCNT with radius greater than 0.7 nm, or largerthan the zone folding limit. It is unclear if they will have astable p0 peak for a certain diameter range. As a whole, p1–p5
peaks trend as expected, particularly above the zone-foldinglimit. Below this limit, some e99(v) peaks (most notably for thechiral geometries) distort and shift in unpredictable ways,underscoring the need to obtain this information for eachSWCNT rather than approximate it using the data of anotherchirality. In contrast, the armchair class of SWCNTs has p1–p5
peaks that vary smoothly down to the smallest diameters. Thesimilar geometry, electronic structure, and symmetry probablycontribute to this resiliency.
Like p0, the s peaks are typically invariant as a function ofradius within a given SWCNT class for diameters above thezone-folding threshold. Up to three s peaks are typicallyidentified. The s0 peak tends to be around 14.5 with a sister s1
peak around 13 eV. Armchair SWCNT geometries have anothermore rounded peak around 27 eV whereas the zigzaggeometries do not. The remaining peaks that arise for verysmall diameters are not readily named with this systembecause they can be sharp, often contain only a limited areaunder the curve, and are difficult to compare tube to tube.With a coarser resolution in the e99(v) data (e.g., 0.05 eVinstead of 0.01 eV), many of these peaks simply disappear. Wecollectively name these s* because their significance dependson the context of the question to be answered.
For the s peaks, the armchair SWCNTs have values of s0
and s1 of 14.56 and 13.45 (14.56 and 12.69) respectively in theaxial (radial) direction. Thus the location of the s0 peak is thesame for both directions and the s0 shifts roughly 0.8 eV. Forthe zigzag chirality (metal and semiconducting), the s0 peak’slocation is also at 14.56 for both directions. But the s1 peakscorrespondingly shift about 0.1 eV to 13.60 and 12.83 for theaxial and radial directions, respectively. These shifts may seemsmall, but changes in position for peaks having large areas
Fig. 6 (a) e99(v) optical dispersion spectrum around 0 eV for eight zigzag SWCNTs spanning a large range of diameters. (b) A log-log plot of e99(v) versus energy forfive zigzag metals. The data below 0.1 eV begins to express a flat slope of 22, indicating a divergent behavior down to 0 eV. Frequency in eV.
832 | RSC Adv., 2013, 3, 823–842 This journal is � The Royal Society of Chemistry 2013
Paper RSC Advances
under the curve could have a large impact on vdW–Ldinteraction.
Thus far, our primary focus has been on trends of thedispersion properties of a large population of categorizedSWCNTs. At the small-diameter limit, there are no stable p0 ors0 peaks, and the rest of the peaks can vary in unpredictableways. Increased curvature introduces more sp3 hybridization,causing the electronic structure to depart strongly from that ofgraphene.30 Also, the large decrease in cutting line densitymeans that the allowed states within a given BZ are quitedifferent. Large optical dispersion variability is found whenthe different electronic structures are combined with thedifferent allowable samplings. This is illustrated in Fig. 7,which shows the e99(v) spectra of four very small diameterchiral tubes in the p and s regions.
4 General observations on the opticalproperties of SWCNT
Perhaps the most important contribution from the aboveanalysis is the quantification of the variations of e99(v) in the0.0–0.1, 0.1–5, and 5–30 eV ranges. The basic trends that occurin the 0–5 eV range are established in the literature. Theoptical dispersion properties in this range are mostlycorrelated with electronic structure, which depends on thecutting line position (i.e., whether the K-points are crossed)and the packing density (which shifts the peaks toward oraway from 0 eV based on the distance of the cutting lines fromthe K-points). The only major departure from the previouselectronic studies is that of the M0 regime. Here we discoveredthat some metals (notably armchair SWCNTs) do not exhibit astandard metal peak despite having the available valence andconduction band states. This results in the metal paradoxwhere the armchair metals are optically like semiconductors.70
In contrast to the M and p regimes, the optical properties inthe 5–30 eV range are largely dictated by the effect ofunderlying geometry on band to band transitions at higherenergy. This means all zigzag SWCNTs at the large diameter
limit will have identical properties above 5 eV despite havingdistinct behaviors (i.e., null, M1, or M0 metal peaks and metalversus semiconducting p peaks) in the lower energy regimes.
Having extended our focus beyond DOS and electronicstructure, the interesting symmetry considerations outlined byDresselhaus, Saito et al. do not necessarily manifest them-selves as notable differences in the optical properties.9 Certainoptical transitions are symmetry forbidden, unlike the analysisof Katura plots and the VB to CB transition tracking withradius.79 This is a hazard of stopping at the DOS level analysisand approximating the optical properties without explicitlycalculating the dipole matrix elements. For example, theknown differences (metal versus semiconducting position ofp1) and trends (p1–p5 shifting with radius) lead to easilyobservable differences in key optical properties, such as theindex of refraction. In the small diameter limit (where theaforementioned trends have broken down) SWCNTs like the[6,2,s], [6,1,s], and [5,1,s] have little correlation in the e99(v)peaks leading to a distinct set of properties for each of thesesmaller tubes. Such variations are important for materialselection and experimental design. While we cannot makebroad predictions without performing calculations, the calcu-lations for vdW–Ld interactions should be straightforward andcan be used to find the relevant variations (see below).
Our new classification is different from the existing ones,both in terms of the particular categories selected and thereasons for their selection. For example: Lambin et al. correctlymoved beyond the simple zone-folding classification byidentifying the armchair metals as true metals while ascribingvery small gap semiconductor characteristics to chiral andzigzag metals.19 But it is the armchair that behaves opticallylike 1+ eV semiconductors. The zigzag and chiral semimetalswith their sub 0.05 eV band gaps exhibit some form of a metalpeak. Thus the division between armchair and non-armchairSWCNTs is correct, but the correlation is opposite fromexpectation. The Dresselhaus/Saito system, despite havinginteresting geometry and symmetry considerations relatingdirectly to (n,m), appears to be less accurate as a categorization
Fig. 7 e99(v) optical dispersion spectrum in the (a) 0–5 and (b) 10–20 eV range for four very small, chiral SWCNTs. Frequency in eV.
This journal is � The Royal Society of Chemistry 2013 RSC Adv., 2013, 3, 823–842 | 833
RSC Advances Paper
tool for the optical properties in the range. As an example, theM-2p metal category in this classification contains botharmchairs and chiral metals. But as seen earlier, the metalpeaks of these two groups are different and will lead todifferent vdW–Ld interactions. This discrepancy is a result ofthe zone-folding approximation. Despite these shortcomingsin explaining the e99(v) optical dispersion properties, thedescriptors used to create this classification are useful indescribing more quantitative differences in cutting lineposition, angle, and packing density. Whether some e99(v)optical dispersion properties link with the symmetry differ-entiation contained with this classification can only bedetermined when results on more chiral semimetals andsemiconductors are available. Until then, geometry is still a farmore important parameter for the 0–30 eV optical properties.9
5 Van der Waals–London dispersioninteractions
Represented by the chirality vector (n,m), chiral properties ofSWCNTs are connected with their vdW–Ld interactions thatdepend on their optical properties through the dielectricfunction, e99(v). The Kramers–Kronig transform of e99(v) leadsto the vdW–Ld spectrum (vdW–Lds) e(ij), i.e., the dielectricresponse function at the imaginary values of the frequency j, thatserves as the basic input for the Lifshitz theory of vdW–Ldinteractions.34–36,80 Above, we addressed and discussed in detailthe connection between the chirality vector (n,m) and the opticaldispersion spectra e99(v). While non-intuitive features can occurwhen one tries to categorize the SWCNT properties based on theirelectronic spectra (e.g. the metal paradox for armchair SWCNTs),most of the relationships between the SWCNT atomic structureand geometry and their optical properties are conceptuallystraightforward. We now proceed from electronic structure andoptical properties of SWCNTs to their vdW–Ld spectra and theensuing vdW–Ld interactions connecting chiral properties ofSWCNTs with long-range interactions.
5.1 Van der Waals–London dispersion spectra
Connecting the imaginary part of the dielectric function e99(v)with the corresponding vdW–Ld spectrum, e(ij), the Kramers–Kronig (KK) relation78
e(ij)~1z2
p
ð?0
ve’’(v)
v2zj2dv (2)
describes the connection between material’s response to externalelectromagnetic fields of a given frequency and the vdW–Ldspectrum, which characterizes the magnitude of spontaneouselectromagnetic fluctuations at the frequency j. In general e(ij) isa real, monotonically decaying function of the imaginaryfrequency j.78
Note that the integration in eqn (2) is over an infinitefrequency range. In practice, it is usually impossible to knowthe frequency response of a material accurately over the wholefrequency range. Fortunately this is unnecessary as long as all
the inter-band transition energies determining the opticaldispersion spectrum are either known or properly approxi-mated. The e99(v) at high energies in the optical domain needsto be pronounced in order to contribute to the resulting vdW–Lds in any significant way because of the heavy damping in thedenominator of eqn (2). The SWCNT e99(v) spectra above 30 eVdescribed in this paper were relatively small in magnitude andnoisy. Therefore a cutoff energy of 30 eV was selected to bestachieve the desired accuracy when evaluating the Kramers–Kronig transforms.
There exist distinct counterbalancing effects between highenergy wide peaks or low energy narrow peaks, and becausee99(v) and e(ij) are connected via an integral transform, it ispossible to have identical vdW-Ld spectra with very differentdielectric functions. Furthermore, excitonic effects that modifye99(v) with peak structures50 will have in general only a small effecton e(ij),66 which remains a smooth monotonically decreasingfunction of its argument. In fact, as is clear from eqn (2), everypeak will contribute to the vdW–Ld transform approximatelyadditively, as the area under the peak, scaling inversely with j2, i.e.inversely with the square of the Matsubara frequency. Since it isthe Matsubara frequency summation in the optical regime of thevdW–Ld transform that determines the Hamaker coefficients andthe strength of vdW interactions, see eqn (5) below, thecorresponding excitonic effects on these, while of course present,will be by necessity small. This statement is substantiated by amore detailed quantitative analysis based on full measuredSWCNT optical spectra containing an explicit excitonic part.66
5.2 Hamaker coefficient
The Hamaker coefficient measures the strength of the vdW–Ldinteraction energy between two interacting materials.33,78,81 Itis defined with respect to the geometry or configuration of theinteraction setup and the shape of the interacting bodies. Itsmagnitude depends upon the optical contrast between theinteracting materials and the bathing medium. It varies as afunction of separation, a consequence of retardation. In thelimit of small separations it can be spoken of as a constant. Inwhat follows we shall consider only the vdW–Ld interactions atsuch small separations, either between two parallel SWCNTsor between a single SWCNT parallel to an anisotropic planarsubstrate.34,36
The cases of larger and very large separations between twoSWCNTs and between a SWCNT and a planar substrate havebeen dealt with in our other publications that also contain fullderivations for all separation limits.34,36,82 Our analysis isstrictly applicable only in the limit of infinitely long SWCNTs;for a consistent analysis of finite size effects and ideal metallicstatic dielectric response, one needs to consider an exactgeneral multiple scattering formulation of the vdW–Ldinteractions, such as that derived by Emig and coworkers.83
Consider first the vdW–Ld interaction free energies betweentwo identical infinitely long parallel SWCNTs at small separa-tions, where retardation effects can be neglected.34 We definethe dispersion anisotropy parameter for a cylindrical SWCNT,cc(v), as
834 | RSC Adv., 2013, 3, 823–842 This journal is � The Royal Society of Chemistry 2013
Paper RSC Advances
cc(ij)~ecE(ij){ec
\(ij)
ec\(ij)
, (3)
where ecE,\(ij) are the parallel (with respect to the cylinder axis)
and the perpendicular components of the vdW–Ld spectrum ofthe cylinder. The van der Waals interaction free energy per unitlength between two such parallel SWCNTs of radius a, at aseparation ‘%a, has the form34
(4)
where the sum of coefficients and
, is
z ~3
2
kBT
2p
X?n~0
’ð2p
0
dyD2 ec\,em,c
� �, (5)
with
D ec\,em,cc
� �~
ec\(ijn)
ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi1zcc(ijn) cos2 y
p{em(ijn)
ec\(ijn)
ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi1zcc(ijn) cos2 y
pzem(ijn)
: (6)
Here em(ijn) is the vdW–Ld spectrum of the interveningmedium. The vdW–Ld response functions in above equations
are given at a discrete set of Matsubara frequencies jn~2pkBTn
,
where kB is the Boltzmann constant and B is the Planck constantdivided by 2p. At room temperature, the interval betweenneighboring Matsubara frequencies is approximately 0.16 eV.The prime in the summation signifies that the first, n = 0, term is
taken with weight1
2.
In general at a finite mutual angle of the dispersionanisotropy axes h the vdW interactions are codified by twovalues of the Hamaker coefficient, i.e. and , whereasin the parallel geometry they are given by a single value
z .34,36,82
The most important aspect of the connection between theHamaker coefficients and the magnitude of the vdW–Ldinteractions is the optical contrast, or dispersion mismatchDecÞ ,em,cc in eqn (6), essentially proportional to the difference
of the dielectric response function over their sum at everyabrupt dielectric interface. The Hamaker coefficients foranisotropic materials are thus proportional to the angular y
integral of the product of all the dispersion mismatches in thesystem. Clearly, if two materials at each dielectric interface atzero mutual angle have identical dielectric responses at a givenMatsubara frequency, the mismatch term goes to 0 and thereis no contribution to the Hamaker coefficient at that particularfrequency. Thus the magnitude of the Hamaker coefficient isdictated by the degree of dispersion contrast at bothinterfaces. On the other hand, the sign of the interaction (i.e.attraction vs. repulsion) is determined by the sign of thedispersion mismatch at the two interfaces if they are notidentical. Depending on the dielectric response of all themedia involved, the vdW–Ld interaction can have bothsigns.78,84
One also notes that the contributions of the radial and theaxial directions are inherently coupled in the Hamakercoefficients. This means that we cannot simply average theinteractions of the pure axial ec
I and radial ecÞ components,
particularly if there is a large degree of optical anisotropy in agiven material. Optical contrast is thus the root source for vdW–Ld interactions. Geometry determines how that contrast isweighted, while the configuration, or stacking order of thematerials and thereby their vdW–Ld spectra in the calculation,determines the sign. There are additional complexities (e.g.,retardation,36 presence of many walls in the CNTs, surfactantscovering the CNTs,35 etc.), but these topics are beyond the scopeof this paper and have been treated at length elsewhere.78
6 Van der Waals–London dispersion spectra
Of the three types of e99(v) variations: position, shape and areaof the peak, SWCNT vdW–Ld spectra are primarily affected byshifts in p1–p5 dispersion peaks as well as the details of thetype of metal peak. In the first part of this paper we definedand outlined these differences in the electronic structure anddielectric response functions in detail. Here we limit ourselvesonly to the most noteworthy vdW–Ld spectra.
6.1 Armchair SWCNT vdW–Ld spectra
VdW–Ld spectra e(ij) of armchair SWCNTs are the moststraightforward class for several reasons: 1) they have identicalcutting line or chiral angles due to their similar geometricalconstruction, 2) they are all electronic structure metals, 3) theyare all null metals, and 4) pragmatically they are by far theeasiest to calculate. Points 1, 2, and 3 are advantageous. We canfocus solely on the effects of radius before adding additionalfeatures (e.g., metal peaks, metal/semiconductor differences inthe p1–p5 peak positions, etc). Point 4 becomes an issue forchiral SWCNTs, which require a larger number of atoms in theband structure calculation and therefore more computation.
Large diameter armchair SWCNTs have nearly identical s
peaks, no metal peaks, and p1–p5 peaks that shift as a functionof inverse diameter. Thus the resulting vdW–Lds are primarilyaffected by the dispersion properties in the 0.1–5 eV range.Fig. 8 compares e99(v) and e(ij) for the armchair axial and radialdirections of several large diameter SWCNTs. e99(v) and theresulting e(ij) show smooth and systematic trends. Note thedifferent variation in the high/low energy wings of the dispersionspectrum with respect to radius. While the variation of the radialpart of the dispersion spectrum is obviously very different from thevariation of the axial response, the final effect on the vdW–Ldspectra is very similar. Both show a general increase in themagnitude of the low energy wing with increasing radius.
There is a clear difference in the behavior of the radial andthe axial component of the dispersion spectrum for a givenSWCNT, Fig. 8. In our discussion of the optical properties abovewe outlined the notable difference in the p1 position betweenthe electronic structure metals and semiconductors. Briefly, thefirst and subsequent p peaks for an electronic structure metaltypically occur at a much larger energy than in a semiconductorof equivalent radius. The same is true between the axial and
This journal is � The Royal Society of Chemistry 2013 RSC Adv., 2013, 3, 823–842 | 835
RSC Advances Paper
radial directions of the armchair SWCNTs, which behave aselectronic structure metals in the axial direction and semi-conductors in the radial direction. The result is that semi-conducting SWCNTs have their first p peak much closer to 0 eV,resulting in a steeper vdW–Ld spectrum around 0 eV.
As shown above, the regularity in the trends of dispersionpeaks with respect to radius began to break down at SWCNTradii of approximately 0.7 nm (i.e. the zone-folding limit).However this breakdown in behavior of dispersion peaks doesnot entail a corresponding change in the vdw–Ld spectra forsmaller radii tubes. Small changes in the shape of e99(v) are notenough to impact the vdW–Lds. Fig. 8 compares the resultingaxial and radial direction vdW–Ld spectra for the armchairSWCNTs ranging from the [24,24,m] all the way down to the[3,3,m]. These results show that the trends are systematic downto [5,5,m], which has a radius of 0.34 nm or about half thebreakdown diameter size for the dispersion peaks. Therefore,we can expect that other SWCNT classes will exhibit similarresiliency of the systematic trends in the behavior of vdW–Ldsfor smaller diameter SWCNTs. However, SWCNT types that areless symmetric (i.e. chiral semimetals and semiconductors) areless likely to have such clean trends; the larger variation in theirinterband transition peaks in the dielectric function is causedby a more diverse set of atomic structures.
6.2 Metal SWCNT Ld spectra
Metal peaks can contribute strongly to vdW–Ld spectra,Hamaker coefficients, and consequently to total vdW–Ld
interaction energies. According to the classification intro-duced in the first part of this paper, we group the three typesof behavior in the dielectric function that were observed in the0.00–0.10 eV metal regime into null, M0, and M1 classes.Despite this, SWCNTs having a continuous DOS through theFermi level, the armchair SWCNTs have no metal featureswhile the chiral metals exhibit both M0 and M1 metal typepeaks. This is the metal paradox whereby symmetry forbidscertain interband transitions, giving them a vanishing dipolematrix element despite the available conduction to valenceband states.
The divergence of axial vdW–Ld spectra near j = 0 dependsstrongly on both the size and location of the interbandtransition peaks. Thus, for a given peak magnitude and areaunder the curve, an M0 peak would result in a larger vdW–Ldspectral amplitude since its peak in the dielectric function isshifted to 0 eV. However, an M1 peak can still have a largereffect than a M0 peak if its oscillator strength is significantlygreater. One thus cannot directly correlate one dielectricfunction peak with one type of vdW–Ld spectral featurebecause the integral transform between the dielectric functionand the vdW–Ld spectrum. Yet there is a tendency for themetal M0 peaks to contribute more strongly for a given peakheight and area under the peak.
The M0 and M1 axial peaks can sometimes vary system-atically as a function of radius within a given SWCNT type. Inthe first part of this paper, the zigzag type of SWCNTs are
Fig. 8 A comparison of radial and axial e99(v) (top) and vdW–Ld spectrum e(ij) (bottom) variations in the radial and axial directions for armchair SWCNTs, from[15,15,m] to [24,24,m]. Radii and electronic structure (metal, semimetal, semiconductor) of the SWCNTs are listed in Table 1. Frequency in energy units (eV).
836 | RSC Adv., 2013, 3, 823–842 This journal is � The Royal Society of Chemistry 2013
Paper RSC Advances
found to have M0 peaks for the [9,0,m] all the way to the[21,0,m], varying inversely with radius. For zigzag metals largerthan the [21,0,m], the M0 peaks give rise to an M1 peak with amagnitude that eventually became negligible by the [30,0,m]SWCNT, Fig. 9.
In comparison, chiral metals lack the systematic shift in M0
and M1 peaks as a function of radius; consequently their vdW–Lds magnitudes are harder to classify. Additionally, thedifferences in their s and p peak positions as a function oftheir chiral angles result in further changes of spectral featuresacross the entire energy range. Thus the armchair, zigzag, andchiral metals can offer very diverse properties. Fig. 10 showsspecific examples of radial and axial vdW–Ld spectra forsimilar diameter SWCNTs within each structural class.
6.3 Semiconductor SWCNT Ld spectra
Large-diameter zigzag semiconductor SWCNTs are the last ofthe three classes of SWCNTs in which we can observe theeffects of increasing radius while fixing the chiral angle andthus limiting variability in the s interband transition peaks.Obtaining optical properties such as the dielectric function for
very large diameter chiral SWCNTs is still difficult but willlikely become easier with greater computational resources.Fig. 11 compares vdW–Ld spectra for large zigzag semicon-ductor SWCNTs with those of the armchair metal SWCNTs.Because these SWCNTs are semiconducting in the axialdirection, their p1 peak occurs much closer to 0 eV and resultsin a sharper vdW–Lds wing near 0 eV. Because of the lack of ametal peak and a shift of p1 peak out to higher energies, thearmchair metals have a vdW–Lds slope that is comparativelymuch flatter. However, the behaviors of the radial vdW–Ldspectra for these two geometrical types are similar becausetheir p dispersion properties are largely unaffected by therelationship of the cutting lines with the K-point crossings.Variations in the s properties are identifiable but may beineffective as a change in shape versus a change in dispersionspectrum peak-width or position.
In the armchair classification, variations in the dielectricfunction appeared to cancel and result in smoothly varyingvdW–Lds down to the smallest SWCNTs. However, smalldiameter chiral SWCNTs were found to have considerablymore spectral variation because of the changing electronicstructure and cutting line angles. The result is a collection ofvdW-Lds that don’t appear to behave in any systematic ordefinable way. Fig. 12 compares e99(v) and e(ij) of armchairand chiral SWCNTs of varying electronic structure properties.Any correlations are inconsistent and unpredictable. The[6,2,s] and [6,4,s] have nearly identical axial direction e(ij),but differ greatly from [6,1,s], which has an axial e(ij) similarto that of [5,1,s]. While a given pair may have similar axial e(ij),they might still have completely different radial e(ij), and viceversa.
7 Hamaker coefficients
Do these trends in the electronic structure and correspondingvdW–Ld spectra persist to the level of the Hamaker coefficientand vdW interactions? Fig. 13(a) shows the e(ij) Hamakercoefficients derived in sec. 5.2, at small separations for cylinder–cylinder interactions for all 64 SWCNTs across vacuum and water,
Fig. 10 The axial (a) and radial (b) vdW–Ld spectra of SWCNTs representing all three structural types of electronic structure metals: armchair, zig-zag, and chiral.Examples of radial and axial vdW–Ld spectra for similar diameter SWCNTs within each structural class. For details see Table 1. Armchair SWCNT [10,10,m], [11,11,m],zigzag SWCNT [15,0,m], [18,0,m], and chiral SWCNT [8,5,m], [9,3,m]. Frequency in eV.
Fig. 9 Axial e(|j) of zig-zag metals for energies close to 0 eV. The vdW–Ldspectrum e(|j) is obtained from the appropriate e99(v) presented in Fig. 6.Frequency in eV.
This journal is � The Royal Society of Chemistry 2013 RSC Adv., 2013, 3, 823–842 | 837
RSC Advances Paper
using eqn (5) Intricate and systematic variations motivate furtherexamination.
In the limit of large CNT radii, the Hamaker coefficients fordifferent classifications of SWCNTs trail different asymptotes,Fig. 13. The numerical values of the Hamaker coefficients arerelatively flat and unchanging above the zone-folding limitcorresponding to a CNT radius of about 0.7 nm. Below thislimit, their magnitudes begin to shift upward as an inversefunction of diameter. One observes a widening envelope thatencompasses all the variations in the Hamaker coefficients
and becomes larger as the tube radii get smaller. For thesmallest tubes, the difference in the Hamaker coefficients canbe almost an order of magnitude between different classifica-tion types.
The large variation in vdW–Ld spectra as a function of (n,m)results in a substantial variation in the correspondingHamaker coefficients, a result that could not have beenpredicted by the tight binding approximation, electronicstructures classification analysis, force-field modeling, orother approaches other than the explicit determination of
Fig. 11 The (a) axial and (b) radial vdW-Ld spectra for the armchair ([23,23,m], [24,24,m]) and electronic structure semiconducting zig-zag ([28,0,m], [29,0,m])SWCNTs. Radii and electronic structures from Table 1. Note that the vdW–Ld spectra of different types of SWCNTs can cross. Frequency in eV.
Fig. 12 A comparison of radial and axial e99(v) (top) and e(|j) (bottom) for very small diameter armchair ([3,3,m], [4,4,m]) and chiral ([5,1,s], [6,1,s], [6,2,s], [6,4,s])electronic structure semiconducting SWCNTs. The radii and electronic structure of the SWCNTs are listed in Table 1. Frequency in eV.
838 | RSC Adv., 2013, 3, 823–842 This journal is � The Royal Society of Chemistry 2013
Paper RSC Advances
the electronic structure and optical properties and theresulting full spectral Hamaker coefficients.
Hamaker coefficients and vdW–Ld interactions show a widevariation among different CNT types. To simplify we limit thediscussion here to the particular example of two parallelcylindrical SWCNTs at the small separation limit (see ref. 34and 35). A system design example will be included in theremaining two subsections to demonstrate practical usage (seealso the Gecko Hamaker project, http://sourceforge.net/projects/geckopro, a free and open source project that enables thecalculation of full spectral Hamaker coefficients for these andmany other systems).
7.1 Hamaker coefficients and SWCNT properties
Fig. 13(b) compares Hamaker coefficients for various classes:armchair, chiral metals, chiral semimetals, zigzag metals andzigzag semimetals. The Hamaker coefficient behaves system-atically across all individual classes but exhibits substantialvariation between classes. This is not surprising given thevariety of metal and p dispersion peak behavior among thedifferent classes. The larger diameter tubes in Fig. 13(b) have aclear ranking in Hamaker coefficient strength as a function ofspectral class. However, these trends begin to cross over belowthe 0.7 nm zone folding limit, and there is also someadditional noise/variation from the introduction of the chiral
classes. Overall, Hamaker coefficient strengths for theSWCNTs drop by a factor of 2 when the radius decreasesfrom the 0.2 nm to 0.5 nm. For tubes larger than 0.5 nm, thedecrease in Hamaker coefficient continues through the largesttubes examined here.
We cannot completely attribute the larger range of Hamakercoefficient magnitudes in Fig. 13 to the effects of increasingcurvature at the small diameter limit. The large diameter limitrepresents only 3 of the 5 SWCNT categories because of thecomputational difficulty in obtaining very large diameterchiral metals and semiconductors. It is possible that thevariation at this limit will be seen once these last two types areincluded at this diameter limit.
The magnitudes of Hamaker coefficients for larger radiusSWCNTs in no way prevents the ability to separate theseSWCNTs. To separate by class, one would design methods thattarget the different asymptotic limit behavior of the Hamakercoefficients. To separate within a class (perhaps by radius) onewould have to create a Hamaker coefficient that would dividealong the classification, see below.
7.2 Hamaker coefficients and the interaction medium
In Fig. 13(a) we show the corresponding Hamaker coefficientsin water and in vacuo. For all but the smallest SWCNTs, theHamaker coefficients differ systematically by a factor of 2between these two media.
7.3 Hamaker coefficients and SWCNT size
For macroscopic systems, material properties are typicallyindependent of size. However, for small scales the materialproperties and size can be coupled, as is the case here forSWCNTs whose dispersion spectra are connected with theirradii. The same is true at very large diameters, where vdW–Ldspectra and Hamaker coefficients can be again very similar.
For example, the 1% drop in the Hamaker coefficientbetween the [18,18,m] and [24,24,m] SWCNTs is small relativeto the 33% increase in the radius a. However, the vdW–Ldinteraction energy varies as z , eqn (4). This meansthe [18,18,m] and [24,24,m] may have a Hamaker coefficientvariation of only 1%, but the total energy varies by 13%. In short,Hamaker coefficients can act as useful guides to gauge theinteraction strength but they cannot be the sole source forcalculating the total vdW–Ld interaction energy that containsexplicit dependence on the radius of the tube.
Fig. 14 shows Hamaker coefficient multiplied byffiffiffiap
. We seetwo competing effects. As the Hamaker coefficients themselvesdrop as a function of radius and reach an asymptotic behavioraround 0.8 nm radius and above, variation of the Hamakercoefficient multiplied by
ffiffiffiap
, i.e., the total interaction free energy,for each SWCNT type results in a bowl-shaped curve. Theinteraction free energy at a fixed separation between twoSWCNTs can thus be varied either by changing the materials,affecting the Hamaker coefficient directly, or by changing theradius of the SWCNT. However, the SWCNT material propertiesand their radii are coupled. From Fig. 14 one can deduce that inthe small-radius regime changes in the interaction free energy at agiven surface separation are more directly correlated with thechanges in the Hamaker coefficient itself, while for larger radii
Fig. 13 Comparison of Hamaker coefficients, eqn (5), vs. SWCNT radius a (nm)for a cylinder–cylinder interaction at small separations, in vacuo and in water. a)All calculated SWCNTs in vacuo vs. in water. b) Comparing the 5 vdW–Ldclassifications in vacuo. The water dispersion spectrum is canonical, taken fromref. 78.
This journal is � The Royal Society of Chemistry 2013 RSC Adv., 2013, 3, 823–842 | 839
RSC Advances Paper
there is a small difference in the Hamaker coefficients but thechanges in the radius can be big. We term the first type ofbehavior ‘‘material dominated’’ and the second one ‘‘sizedominated’’.
8 Conclusions
We have reviewed e99(v) optical dispersion properties fortransition energies up to 30 eV and Hamaker coefficients ofthe vdW–Ld interactions of 64 SWCNTs. The resulting trendsin the 0–5 eV or p regime were found to depend on the cuttingline position and packing, while the 5–30 eV or s regimedepended largely on SWCNT geometry. We discovered that thetrends as a function of radius tend to break down and becomemore erratic for tubes of radius less than 0.7 nm. The trends,breakdowns, and other interesting results can be categorizedin a new SWCNT classification based on a combination ofelectronic structure, curvature, and geometry. Ultimately, theanalysis here can lead to a further understanding of thechirality-dependent properties of SWCNTs exploitable byvarious experimental means. The use of ab initio methods toobtain realistic directionally dependent optical absorptionspectra for highly complex systems, that are not available byother means,68 can accelerate the study of vdW–Ld interac-tions in these systems.
We discovered that the optical properties for SWCNTs needa new optical dispersion classification scheme in order toadequately group and address certain features that would bepertinent to practical properties. We have classified the sub-groups of SWCNTs with regard to s, p and metal features.These properties determine also the Hamaker coefficients andtotal energies of vdW–Ld interactions in many ways to serve asa basis for novel classification schemes. Standard classifica-tions based on fewer groupings of the properties (e.g. zone-folding and Lambin classifications19) or on symmetry con-
siderations (e.g. Saito/Dresselhaus classification9) would in ouropinion neglect key possibilities in experimental design.Exploiting important differences in the vdW–Ld interactionsof nanoscale objects will allow better separation and place-ment into nanodevices.
Some SWCNT classes may ultimately be redundant (e.g., thechiral zigzag semiconductors) because the differences are notsignificant enough to warrant such fine distinction. Ouroptical dispersion classification is also equally incapable ofpredicting the unique features that occur for the very smallestSWCNTs. For example, it cannot explain why the [5,0,m] is ametal despite having an (n,m) vector that predicts a semi-conductor. When curvature effects become large, the impacton e99(v) becomes too strong to allow for a generalizedcategorization. The optical dispersion classification also failsto explain why the large diameter zigzag metals lose theirmetal features.
There are also other material properties that may requirerevisiting this classification system. The effects of structuralrelaxation,79 phonons,29 bending moments,85 functionaliza-tion,86 the importance of excitonic effects in the opticalspectral calculation51–55 and interlayer coupling35 may in factcause armchair tubes to lose some symmetry and regain alow-energy spike. Furthermore a high transverse electric fieldmay in fact cause the band gaps to open up.71,73,74,87 Theseeffects are well beyond the scope of this paper, but should bekept in mind in order to see if some differentiations areredundant or if new sub-classes need to be formed. Even ifchanges in the metal and p peaks do arise, the more stable s
peaks should still justify the differentiation from at least anoptical property characterization standpoint. Features ofSWCNT dielectric response justify their newly proposeddispersion classification. While most of this analysis wasspecific to SWCNTs, the general concepts described can beapplied to other nano-materials where vdW–Ld spectralproperties can be altered as a function of geometry or othercontrollable parameters.
Acknowledgements
This research was supported by the U.S. Department of Energy,Office of Basic Energy Sciences, Division of Materials Sciencesand Engineering under Award DE-SC0008176 and DE-SC0008068. R. Rajter acknowledges financial support for thiswork by the NSF Grant under Contract No. CMS-0609050(NIRT). W. Y. Ching acknowledges support under DOE AwardDEFG02-84DR45170 during the period 2005 to 2009. Thisresearch used the resources of NERSC supported by the Officeof Science of DOE under contract No. DE-AC03-76SF00098.
The ab initio optical properties for the SWCNTs discussed hereare available at http://www.lrsm.upenn.edu/yfrenchrh/spectral-data.htm, or as part of Gecko Hamaker, the Open Source, cross-platform program for computing van der Waals–Londondispersion interaction energies and full spectral Hamakercoefficients available at http://geckoproj.sourceforge.net/.
Fig. 14 Comparison of Hamaker coefficients multiplied byffiffiffiap
for two rodlikeSWCNT cylinders in the limit of small separations in water. Hamaker coefficientswere calculated using the anisotropic rod–rod close separation result witharmchair vdW–Ld spectra. The interaction free energy, proportional to Hamakercoefficients multiplied by
ffiffiffiap
at a fixed spacing, distinguishes ‘‘materialdominated’’ and ‘‘size dominated’’ behavior for small vs. large radii.
840 | RSC Adv., 2013, 3, 823–842 This journal is � The Royal Society of Chemistry 2013
Paper RSC Advances
References
1 S. Iijima and T. Ichihashi, Nature, 1993, 363, 603.2 D. Bethune, C.-H. Kiang, M. de Vries, G. Gorman, R. Savoy,
J. Vazquez and R. Beyers, Nature, 1993, 363, 605.3 X. Y. Kong and Z. L. Wang, Nano Lett., 2003, 3, 1625.4 C. A. Bessel, K. Laubernds, N. M. Rodriguez and R. T.
K. Baker, J. Phys. Chem. B, 2001, 105, 1115.5 J. P. Kim, B. Y. Lee, S. Hong and S. J. Sim, Anal. Biochem.,
2008, 381, 193.6 A. Srivastava, O. N. Srivastava, S. Talapatra, R. Vajtai and P.
M. Ajayan, Nat. Mater., 2004, 3, 610.7 Y. Hayamizu, T. Yamada, K. Mizuno, R. C. Davis, D.
N. Futaba, M. Yumura and K. Hata, Nat. Nanotechnol.,2008, 3, 289.
8 J. Kong and H. Dai, J. Phys. Chem. B, 2001, 105, 2890.9 E. B. Barros, A. Jorio, G. G. Samsonidze, R. B. Capaz, A. G.
S. Filho, J. Filho, G. Dresselhaus and M. S. Dresselhaus,Phys. Rep., 2006, 431, 261.
10 X. Y. Kong and Z. L. Wang, Nano Lett., 2003, 3, 1625.11 C. A. Bessel, K. Laubernds, N. M. Rodriguez and R. T.
K. Baker, J. Phys. Chem. B, 2001, 105, 1115.12 J. P. Kim, B. Y. Lee, S. Hong and S. J. Sim, Anal. Biochem.,
2008, 381, 193.13 A. Srivastava, O. N. Srivastava, S. Talapatra, R. Vajtai and P.
M. Ajayan, Nat. Mater., 2004, 3, 610.14 Y. Hayamizu, T. Yamada, K. Mizuno, R. C. Davis, D.
N. Futab, M. Yumura and K. Hata, Nat. Nanotechnol., 2008,3, 289.
15 J. Kong and H. Dai, J. Phys. Chem. B, 2001, 105, 2890.16 V. Popov, Mater. Sci. Eng., R, 2004, 43, 61.17 J. W. Mintmire, J. Phys. Chem. B, 2005, 109, 52.18 I. Cabria and J. W. Mintmire, Phys. Rev. B: Condens. Matter,
2003, 67, 121406.19 P. Lambin, C. R. Phys., 2003, 4, 1009.20 A. Hirano, T. Tanaka, Y. Urabe and H. Kataura, J. Phys.
Chem. C, 2012, 116, 9816.21 S. R. Lustig, E. D. Boyes, R. H. French, T. D. Gierke, M.
A. Harmer, P. B. Hietpas, A. Jagota, R. S. McLean, G.P. Mitchell, G. B. Onoa and K. D. Sams, Nano Lett., 2003, 3,1007.
22 S. R. Lustig, C. A. Jagota and M. Zheng, J. Phys. Chem. B,2005, 109, 2559.
23 M. Zheng, A. Jagota, M. S. Strano, A. P. Santos, P. Barone, S.G. Chou, B. A. Diner, M. S. Dresselhaus, R. S. Mclean, G.B. Onoa, G. G. Samsonidze, E. D. Semke, M. Usrey and D.J. Walls, Science, 2003, 302, 1545.
24 M. Zheng and E. D. Semke, J. Am. Chem. Soc., 2007, 129,6084.
25 S. M. X. Tu, A. Jagota and M. Zheng, Nature, 2009, 460, 250.26 Y. Yan, M. Chan-Park and Q. Z. Q, Small, 2007, 3, 24–42.27 V. Popov, Mater. Sci. Eng., R, 2004, 43, 61.28 M. S. Dresselhaus, G. Dresselhaus, R. Saito and A. Jorio,
Phys. Rep., 2005, 409, 47.29 M. S. Dresselhaus and P. C. Eklund, Adv. Phys., 2000, 49,
705.30 J. C. Charlier, X. Blase and S. Roche, Rev. Mod. Phys., 2007,
79, 677.31 J. Chung, K. H. Lee, J. Lee and R. S. Ruoff, Langmuir, 2004,
20, 3011.
32 H. Peng, N. Alvarez, C. Kittrell, R. H. Hauge and H.K. Schmidt, J. Am. Chem. Soc., 2006, 128, 8396.
33 R. French, V. Parsegian and R. Podgornik, Rev. Mod. Phys.,2010, 82, 1887.
34 R. F. Rajter, R. Podgornik, V. A. Parsegian, R. H. Frenchand W. Y. Ching, Phys. Rev. B: Condens. Matter Mater. Phys.,2007, 76, 045417.
35 R. F. Rajter, R. H. French, R. Podgornik, W. Y. Ching and V.A. Parsegian, J. Appl. Phys., 2008, 104, 053513.
36 A. Siber, R. Rajter, R. French, W. Ching, V. Parsegian andR. Podgornik, Phys. Rev. B: Condens. Matter Mater. Phys.,2009, 80, 165414.
37 O. Stephan, D. Taverna, M. Kociak, K. Suenaga, L. Henrardand C. Colliex, Phys. Rev. B: Condens. Matter, 2002, 66,155422.
38 R. H. French, J. Am. Ceram. Soc., 2000, 83, 2117.39 F. Wooten, Optical Properties of Solids, Academic Press, New
York, 1st edn 1972.40 R. F. Rajter, R. H. French, W. Y. Ching, W. C. Carter and Y.
M. Chiang, J. Appl. Phys., 2007, 101, 054303.41 C. T. White and J. W. Mintmire, J. Phys. Chem. B, 2005, 109,
52.42 A. G. Marinopoulos, L. Reining and A. Rubio, Phys. Rev. B:
Condens. Matter Mater. Phys., 2008, 78, 235428.43 P. Nikolaev, M. J. Bronikowski, R. K. Bradley, F. Rohmund,
D. T. Colbert, K. A. Smith and R. E. Smalley, Chem. Phys.Lett., 1999, 313, 91.
44 D. E. Resasco, W. E. Alvarez, F. Pompeo, L. Balzano,J. Herrera, B. Kitiyanan and A. Borgna, J. Nanopart. Res.,2002, 4, 131.
45 V. Popov and L. Henrad, Phys. Rev. B: Condens. MatterMater. Phys., 2004, 70, 115407.
46 W.-Y. Ching and P. RulisElectronic Structure methods forComplex Materials, The Orthogonalized Linear Combinationof Atomic Orbitals, Cambridge University Press, OxfordUniversity Press, 1st edn 2012.
47 H. Ehrenreich and M. Cohen, Phys. Rev., 1959, 115, 786.48 R. F. Rajter and R. H. French, J. Phys.: Conf. Ser., 2008, 94,
012001.49 G. Lanzani and L. Ler, in Comprehensive Nanoscience and
Technology, Elsevier, 2010, vol. 1, p. 2339.50 M. S. Dresselhaus, G. Dresselhaus, R. Saito and A. Jorio,
Annu. Rev. Phys. Chem., 2007, 58, 719.51 C. Spataru, S. Ismail-Beigi, L. Benedict and S. Louie, Phys.
Rev. Lett., 2004, 92, 077402.52 P. Trevisanutto, C. Giorgetti, L. Reining, M. Ladisa and
V. Olevano, Phys. Rev. Lett., 2008, 101, 226405.53 L. Yang, J. Deslippe, C.-H. Park, M. L. Cohen and S. Louie,
Phys. Rev. Lett., 2009, 103, 186802.54 P. Gudazzo, C. Attaccalite, L. V. Tokatly and A. Rubio, Phys.
Rev. Lett., 2010, 104, 226804.55 G. Luo, X. Qian, H. Liu, R. Qin, J. Zhou, L. Li, Z. Gao,
E. Wang, W.-N. Mei, J. Lu, Y. Li and S. Nagase, Phys. Rev. B:Condens. Matter Mater. Phys., 2011, 84, 075439.
56 T. Ando, J. Phys. Soc. Jpn., 1997, 66, 1066.57 C. L. Kane and E. Mele, Phys. Rev. Lett., 2003, 90, 207401.58 V. Perebeinos, J. Tersoff and P. Avouris, Phys. Rev. Lett.,
2004, 92, 257402.59 T. Pedersen, Carbon, 2004, 42, 1007.60 E. Chang, G. Bussi, A. Ruini and E. Molinari, Phys. Rev.
Lett., 2004, 92, 196401.
This journal is � The Royal Society of Chemistry 2013 RSC Adv., 2013, 3, 823–842 | 841
RSC Advances Paper
61 J. Maultzsch, R. Pomraenke, S. Reike, E. Chang andD. Prezzi, Phys. Rev. B: Condens. Matter Mater. Phys., 2005,72, 241402.
62 J. Wang, G. Dukovic, L. Brus and T. Heinz, Science, 2005,308, 838.
63 J. Jiang, R. Saito, G. G. Samsonidze, A. Jorio, S. Chou,G. Dresselhaus and M. S. Dresselhaus, Phys. Rev. B:Condens. Matter Mater. Phys., 2007, 75, 035407.
64 P. Avouris, M. Freitag and V. Perebeinos, Nat. Photonics,2008, 2, 341.
65 J. Lefebvre and P. Finnie, Nano Res., 2011, 4, 788.66 E. Hobbie, T. Ihle, J. Harris and M. R. Semler, Phys. Rev. B:
Condens. Matter Mater. Phys., 2012, 85, 245439.67 P. Loskill, H. Hahl, T. Faidt, S. Grandthyll, F. Muller and
K. Jacobs, Adv. In Colloid and Interface Sci., 2012, 179–182,179.
68 L. Liang, P. Rulis, B. Kahr and W. Ching, Phys. Rev. B:Condens. Matter Mater. Phys., 2009, 80, 235132.
69 L. Liang, P. Rulis, L. Ouyang and W. Ching, Phys. Rev. B:Condens. Matter Mater. Phys., 2011, 83, 024201.
70 R. F. Rajter, PhD thesis, MIT, 2009.71 Y. Li, S. V. Rotkin and U. Ravaioli, Nano Lett., 2003, 3, 183.72 Y. Li, S. V. Rotkin and U. Ravaioli, Appl. Phys. Lett., 2004,
85, 4178.73 Y. Li, U. Ravaioli and S. V. Rotkin, Phys. Rev. B: Condens.
Matter Mater. Phys., 2006, 73, 035415.74 Y. Li, S. V. Rotkin and U. Ravaioli, Proc. IEEE Nanotechnology,
2003, 3, p. 1.
75 E. M. Lifshitz, Sov. Phys. JETP, 1956, 2, 73.76 H. B. G. Casimir and D. Polder, Phys. Rev., 1948, 73, 360.77 S. J. Rahi, T. Emig, R. L. Jaffe and M. Kardar, Phys. Rev. A:
At., Mol., Opt. Phys., 2008, 78, 012104.78 V. Parsegian, Van der Waals Forces, Cambridge University
Press, Cambridge, 1st edn, 2005.79 G. G. Samsonidze, R. Saito, N. Kobayashi, A. Gruneis,
J. Jiang, A. Jorio, S. G. Chou, G. Dresselhaus and M.S. Dresselhaus, Appl. Phys. Lett., 2004, 85, 5703.
80 J. Sarabadani, A. Naji, R. Asgari and R. Podgornik, Phys.Rev. B: Condens. Matter Mater. Phys., 2011, 84, 155407.
81 M. Bordag, G. L. Klimchitskaya, U. Mohideen and V.M. Mostepanenko, Advances in the Casimir Effect, OxfordUniversity Press, Oxford, 1st edn 2009.
82 A. Siber, R. Rajter, R. French, W. Ching, V. Parsegian andR. Podgornik, J. Vac. Sci. Technol., B: Microelectron.Nanometer Struct.–Process., Meas., Phenom., 2010, 28,C4A17.
83 T. Emig, N. Graham, R. L. Jaffe and M. Kardar, Phys. Rev. D:Part., Fields, Gravitation, Cosmol., 2008, 77, 025005.
84 J. N. Munday, F. Capasso and V. A. Parsegian, Nature, 2009,457, 170.
85 J. Bernholc, D. Brenner, M. B. Nardelli, V. Meunier andC. Roland, Annu. Rev. Mater. Res., 2002, 32, 347.
86 C. Richard, F. Balavoine, P. Schultz, T. W. Ebbesen andC. Mioskowski, Science, 2003, 300, 775.
87 Y. Li, S. V. Rotkin and U. Ravaioli, Appl. Phys. Lett., 2004,85, 4178.
842 | RSC Adv., 2013, 3, 823–842 This journal is � The Royal Society of Chemistry 2013
Paper RSC Advances